**Chapter 1. Thermonuclear Fusion**

**2.1.5. Non-simple metals: the s-p interaction**

The function Yi is integrated over the spherical Fermi surface (as we are considering a simple alloy) with diameter 2kF, and it contains the structure factor and the form factor in which the transition probability matrix can be decomposed when pseudopotential (w(r)) approximation is applied (see further section 2.1.5). Yi is an oscillating function which depends on q and decays as i grows, thus is clear that only first few coordination shells will play a role. Depending on the material even the resistivity could be proportional to the linear combination of first and second SRO parameters, α12.

It has been shown that the presence of migrating defects enhances changes in SRO parameters leading to changes of residual resistivity. Typically such investigations have been done by means of quenching experiments. Such experiments consist on the creation of thermal vacancies by heating up the samples (up to the so-called quenching temperature Tq) followed by an extra-fast cooling up to the annealing temperature at which isothermal annealing is going to be performed. The excess of thermal vacancies created by quenching are able to migrate within the material and the residual resistivity values which are monitored are shown to change. Changes in ρ0 are due to re-arrangement of solutes enhanced by the presence of migrating vacancies. This phenomenon is also going to occur in our measured Fe-Cr samples as the RR experiments will be run. Thus this effect will have to be taken into account when analysing the data. Much research has been done on SRO kinetics using quenching and irradiation experiments [48–54] in concentrated alloys but no works have been found in the study of Fe-Cr alloys.

Fig. 2-5: Scheme of pseudopotential approximation (red, continuous line) vs. real part of true wavefunction in the presence of Coulomb potential (blue, dotted line).

In non-simple alloys it is assumed that most of the current is carried by the electrons in the “s-band”, because of the value of its effective mass (close to that of electrons in copper, Mott and Jones 1936), while the “d-electrons” have much higher effective mass and therefore much lower mobility (see equation 2-12). Impurities, phonons and electron-electron interactions will cause scattering of the s electron-electrons into vacant s- and d- states, but since the scattering probability depends upon the density of states into which the electrons are scattered (equation 2-13), s-d scattering mechanisms occurs much more frequently than s-s scattering. Electrons scattered into de “d-band” increase the resistivity because of their increased effective mass. The importance of the density of states in the d-band can also lead to a modification of the temperature dependence of the resistivity, given by a rapid increase of Nd(EF) with temperature. Such effect would lead to an additional temperature dependent term [46] with respect to equation 2-15:

'
" ' '
^{} '
2-26
If we now look at the residual resistivity value of non-simple alloys, it has come clear
that the s-d scattering probability has to be taken into account. At this point some
qualitative understanding of this phenomenon is possible under the rigid band model. The
following explanation is based on empirical observations on the system Ag-Pd. Let’s
assume in general a transition metal A which has an s-band similar to that of B transition
metal and also a narrow d-band which overlaps the s-band and EF near the top of d-band.

Then as B metal is added to A, the s-electrons of B atoms are supposed to fill the d-band leading to a decrease in Nd(EF) until the d band is filled at ci concentration of B. The density of states of the unfilled d-band can be described approximately as:

7#
~D D
^{}, DS D 2-27
If the atoms are randomly distributed (no SRO effects) an average lattice potential can be
described from the constituent ion potentials of the alloy. This is called the virtual crystal
approximation:

〈!〉 " D! D! 2-28

Such potential can be described by analogy to equation A-18 (see Appendix A) as

! " !T !^{}, where V^{d} is the difference potential. The probability of scattering from an
s-state to a d-s-state is given by:

IN!^{}dSN^{}NE
2-29

The magnitude of scattering potential at a A atom site is cAV^{d} (cf. Rossiter 4.67 [16]) and
the fraction of such sites is (1 - cA) = cB. The scattering probability is thus proportional to:

D D
^{}D_{}^{}D 2-30

If we assume independent contributions from s-s and s-d scattering, as s-s interaction has been determined in the previous section (equation 2-23), then the total residual resistivity might be written as:

' " ρ ρ∝ DD[\F^{}

7 G D^{}EH

] ^D D
^{}D_` 2-31

2.1.6. Magnetic effects and deviations from Matthiessen’s rule: the two current model

Some complications can arise when the non-simple alloy under study is magnetic or
nearly magnetic material as it is the case of the Fe-Cr system, and therefore need to be
considered. Iron, which is the host material, is ferromagnetic (alignment of spins in a
parallel array) whilst the solute, chromium, is antiferromagnetic (alignment of spins in an
antiparallel array). In transition metals the orbital angular momentum of the electrons is
almost zero^{10}, so only the spin magnetic moment of the electrons which are in incomplete
shells contribute to the magnetic moment. It is believed that the inversion of SRO
parameters at Cr concentrations of about 10% is due to some magnetic frustration effect
of the Cr spins, but we will discuss further this question in chapter 4.

When thinking about energy distribution of conduction electrons, their alignment is governed by a special type of interaction known as the exchange interaction which the determines that the energy of electron states is a minimum when the electrons line up with their spins parallel provided that the Pauli exclusion principle is not violated. As a result, there will be different populations of spin-up (↑) and spin-down (↓) conduction electrons which create a dipole moment. Qualitative picture for Fe conduction electrons is represented in Fig. 2-6, from Campbell and Gomès (1967) [55]. It has been confirmed that scattering of spin ↑ is different than the scattering of spin ↓ electrons. Thus a new model has been adopted to understand the electrical resistivity in ferromagnetic materials which also justifies the large deviations on the Matthiessen’s rule which were mentioned in section 2.1.3. The resistivity can no longer been understood as an effect produced by an electron current but by two currents, one referred to spin ↑ and the other to spin ↓. The two-current (or two-band) model is based on the suitable definition of the function ϕk in

10 This effect is usually termed “quenching” of the orbital angular momentum and it means that when the ion is in the crystal there is no orbital magnetic momentum.

the variational method of Köler (cf. Appendix A, Ziman 1960 [56] or Fert and Campbell 1967 [47]) as a linear combination of two functions each of them associated to a certain carrier type, σ = ↑, ↓:

ϕ_{}" G η_{}^{ᇲ}ϕ_{}^{ᇲ}δ_{}^{ᇲ}

^{ᇲ}

2-32 Such differentiation of the distribution function for every spin type in the Boltzmann equation leads to an expression of the resistivity based on the independent (and conveniently defined [47]) resistivity terms for elastic scattering of spin ↑ electrons, ρ↑, and spin ↓, ρ↓, respectively, and an spin mixing term, ρ↑↓:

ρ "ρ↑ρ↓ ρ↑↓ρ↑ ρ↓

ρ↑ ρ↓ 4ρ↑↓ 2-33

The Matthiessen’s rule is applicable to ρ↑, ρ↓ and ρ↑↓ given that every term depends linearly on their scattering operator:

' " ' ' 2-34

'↑↓ " '↑↓ '↑↓ 2-35

Fig. 2-6: The usually adopted band model for iron consists of an almost filled ↑ spin sub-d-band and half filled ↓ spin sub-d-sub-d-band.

In the absence of spin-flip collisions ρ↑↓ cancels out and the resistivity is expressed in a model where the current is carried by two independent currents:

ρ " ρ↑ρ↓

ρ↑ ρ↓ 2-36

The inelastic scattering (spin mixing) occurs by collisions with spin waves and collision between spin ↑ and spin ↓ electrons. Both processes contribute to the temperature dependent term of the resistivity ρ↑↓(T) but the second one can be neglected. The residual term also contains a spin-flip mechanism that contributes to resistivity, ρ0↑↓, which is induced by impurities in dilute alloys and can also be neglected in such cases. As it has been deduced in some experimental works [57], the spin-mixing term can no longer be neglected when impurity contents rise and alloys start no to be dilute any longer. In

chapter 6 we will provide a discussion on the influence of this term in the studied Fe-Cr alloys which we have been able to deduce form residual resistivity measurements.

The two-current model has provided justification for experimental observations in residual resistivities in dilute alloys [58–60]. The parameter α has been conveniently re-defined based on the concepts included in equations 2-33 to 2-36, are used for characterization and quantitative analysis of alloys residual resistivity. Parameter α describes the relation between the resistivity contributions of spin-down and spin-up resistivities:

α "ρ↓

ρ↑ 2-37

Fert and Campbell [58], applied the two current model to calculate the residual resistivity of ternary alloys. The application of such developments allowed unambiguous calculation of αi parameters, from experimental data. The sub-index i refers to a specific solute in the pure host metal. Such development was also applied by Maury et al. to explain the apparent solute specific resistivity in metals (this will be shown in chapter 4 and 5) [37,57]. The development of the model goes as follows. Assuming that spin-mixing term can be neglected (eqn. 2-36) the resistivity of a binary alloy, MA, is:

'" DD '↑'↓

'↑ '↓ 2-38

where cM and cA are the concentrations of M host metal and A solute respectively. If the alloy is dilute, i.e. cA << cM the residual resistivity can be approximated to:

'" D '↑'↓

'_{↑} '_{↓} 2-39

In the case of a ternary dilute alloy, MAB, the Matthiessen’s rule is obeyed for each current, and the impurities A and B add their resistivity in each current (ρσ = cA·ρAσ + cB·ρBσ). Combining such form with equations 2-36, 2-39 and αi=ρi↓/ρi↑ it gives:

∆' " ' ' '
" E E
^{}''

1 E
^{}E' 1 E
^{}E' 2-40

The study of ternary alloys has been of interest because it allowed unambiguous experimental calculation of αi values [58]. Sometimes the systems under study are treated as ternary alloys when besides of the specific solute A, there is another element that can be treated as an impurity, such as created irradiation defects [37,57], o phonons created by the effects of non-zero temperature [59].

Further re-definition of α parameter as it follows [57]:

is going provide double advantage. On one hand it will be possible re-express the residual resistivity of binary alloys including the spin-mixing term, ρ↑↓ = ρm (eqn. 2-33) as:

ρMA
" ρ_{} ρ_{}

1 1 z^{}
ρ^{}iρ_{} 2-42

and this will allow the analysis of the apparent Cr specific resistivity in our Cr alloys (in chapter 5). On the other hand, the development of the two-current model formalism for the study of the radiation induced resistivity reveals that the specific resistivity of the Frenkel pairs (FPs) can be expressed as a function of z and no longer on the defect concentration:

'∗ " 'j1 k k
^{}

1 k_{}^{}
l 2-43

The last concepts just mentioned such as radiation induced resistivity, specific resistivity of FPs are explained in the next section, concerning the radiation effects on the resistivity. The discussions concerning the influence of FP specific resistivity in RR experiments of Fe-Cr alloys and description of the zF (in eqn. 2-43) are provided in chapters 4 and 5.

### Radiation effects on resistivity 2.2.

Once it has been understood how the characteristics of concentrated Fe-Cr alloys are going to influence their electrical conductivity at low temperatures, let’s have a look on how radiation is going to affect the microstructure of the alloys and eventually its resistivity, which is one of the main objectives of this work.

In general the electron and proton irradiations are going to produce simple defects,
i.e. FPs made of a vacancy and an interstitial atom^{11}. At low concentrations (~ppm range)
it is assumed that every FP increases the resistivity of the alloy by a certain amount
(typically measured in μΩ cm at.%). This change in resistance is mainly due to an increase
of the residual resistivity of the metal. Some changes in the thermal component, ρ(T),
occur as well, but since the thermal component is poorly known and small and is difficult
to estimate theoretically, irradiations and measurements are usually made at sufficiently
low temperature to avoid the problem. As the residual resistivity is very sensitive to the
presence of imperfections (as explained in previous sections) its change is then the
appropriate measurement of the generated defect concentration. The residual resistivity
can be monitored during irradiation in order to measure the radiation induced resistivity
(RIR), Δρ, which has a linear relation with the particle fluence in the low dose regime [31].

The RIR is given by:

11 Indeed a study on the type of damage and FP distribution of the irradiations with 5 MeV protons performed in this work will be given in the chapter devoted to experimental results.

k "ρ↓ ρ↑

ρ_{↓} ρ_{↑}"α 1

α 1 2-41

m' " '%n 2-44 where ρF is the specific resistivity contribution of a simple Frenkel defect, σD is the defect production cross-section and Φ is the particle fluence. The defect population created, n, is determined by the product of the creation cross-section and the fluence of irradiating particles. The resistivity of the FP can be described as a sum of discrete contributions from the vacancy, ρv, and the interstitial, ρi, respectively:

m' " ' " 'D ' D 2-45

Thus this physical property is sensitive to both types of defects and separable monitoring of their populations should be possible although very difficult. This feature represents an advantage with respect to other techniques such as positron annihilation (PA) spectroscopy given that they are only sensitive to vacancies.

The study of RIR has been extensively performed; at very low energies and doses it allowed the measurement of threshold energies for FP creation for different materials in the principal crystal directions [22,61] also RIR studies have been used to measure defect production cross-sections and damage efficiency [31]. This last experiments revealed than at high doses intra-cascade recombination decreased the damage efficiency whereas at high mean PKA energies sub-threshold elastic effects and electronic excitations start to play a role. The RIR measurements made in this work (in 5%Cr, 10%Cr and Fe-14%Cr) confirm that the increase in resistivity with fluence is very close to linear so the physics underlying match very well with the previous explanation.

### Annealing theory 2.3.

The annealing is the process of disappearance of the defects which are in the material in excess of the thermodynamic equilibrium. When performing a particle irradiation or a quenching experiment (high temperature heat-up followed by abrupt freezing), we are producing a so-called super-saturated crystal. In such crystals there is a thermodynamic driving force that tends to reduce the defect concentration. At suitable temperature intervals the defect mobility becomes significant. The disappearance of the defects is then experimentally observable and it is associated to migration to sinks (such as dislocations and other internal or external surfaces) or to recombination with complementary defects (e.g. interstitial-vacancy annihilation). In the case of defect clusters, its disappearance is mostly due to dissociation into smaller more mobile defects which eventually recombine.

2.3.1. Defect diffusion

The point defects created in a solid become mobile at sufficient high temperature. The events that they can perform as a consequence of the temperature of the system are diffusion jumps, dissociation from clusters or interact with other defects or impurities.

The thermal motion of the defects is going to provide them some probability to jump over a potential barrier/saddle point from one equilibrium position to another. A statistical mechanics treatment of the problem [62] let show that the probabilities of these events

are given by the migration and binding energies. It is well known that the individual defect jump rate, i.e. the probability for a defect to undergo one migration jump (K), is proportional to the effective vibration frequency (K0) and its migration energy (EM):

o " o^{!"}^{ಾ}^{$ %}^{ #} 2-46

being k the Boltzmann’s constant and T the absolute temperature. If the considered jump involves not only migration but also dissociation from a trap (cluster or impurity) then the jump rate also includes the binding energy (EB):

o " o_{}!"&^{ಾ}'(ా)

$ % # 2-47

These type of expressions which relate a rate exponentially to the reciprocal of the absolute temperature, are often referred to as Arrhenius equation.

The diffusion coefficient is related to the jump rate as:

D " δaΓ 2-48

where δ is a geometrical constant and a0 the lattice parameter.

When studying close to real materials, all the different defects together with their different interactions and diffusion rates need to be calculated simultaneously. This involves non-simple analytical solutions but more complex models and computational approaches that are indicated in next section.

2.3.2. Rate theory

Pure atomistic treatment of the defect kinetics in solids, as kinetic Monte-Carlo, where the
diffusion of every atom is considered individually, is very limited approach from the point
of view of simulations given that it does not allow to simulate macroscopic systems but
only cells on the order of nm (10^{3}-10^{6} atoms) and thus no extrapolation can be applied to
real physical systems. A formalism based on rate equations, where the study is made over
mean concentrations of defects which obey the suitable jump rate for every specific
reaction, is allowing simulations of macroscopic systems with current computational tools
and also sets a mathematical base to interpret indirectly observed defect kinetics in
resistivity experiments. In the rate theory formalism [62,63], the reactions between
defects are supposed to occur via binary reactions of the type:

? s'

s⇌*

F 2-49

where KA+B is the forward constant rate of diffusion of the reactants A and B and KC is the backward constant rate. Constant rates are directly proportional to the diffusion coefficients of the species involved. The law of mass action is fulfilled for this reaction and thus the time evolution of the mean concentration of each species (ci with i=A, B, C) can be describe by the partial differential equation:

*F

*- " s^{'}DD s+D* 2-50

Thus the time evolution of the system is governed by a set of nonlinear coupled partial differential equations which when solved will describe the complete annealing behavior of the system. In some special very simple system descriptions, solutions can be found easily and simulations of time evolution of defect concentrations can be depicted. As an example Fig. 2-7 shows the variation of vacancy (V1), interstitial (i) and trapped-interstitial (C) with impurities (I) concentrations with time in a system which considers vacancy-interstitial annihilation plus interstitial trapping at impurities also described as:

V s,^{భ}'

→ >vw>-@ 2-51

xs-'.

s⇌*

F 2-52

Fig. 2-7: Plot of the defect populations calculated in the simple system i-V annihilation with
trapping of interstitials by impurities. They are also indicated parameters used for the
calculations: annealing temperature (T), migration energy (Ei), binding ener gy (B), initial
impurity concentration (I^{0}) and initial concentrations of i and v (V^{1}^{0} and i^{0}). Plot taken from

reference [62].

It is important to set the basis for a good qualitative understanding of the subsequent analysis of resistivity recovery results and to describe the fundamental annealing processes in which the rate equations are based. The migrating defect can either diffuse randomly until it disappears on a sink or it reacts with another impurity or defect leading to annihilation or clustering. The following is a short review of these 3 processes.

Random diffusion to sinks

This is the simplest process in which the mobile species diffuse to a fixed number of unfillable sinks (dislocations, grain boundaries or external surfaces). The long-time solution is always a simple exponential decay and it can be shown by rate theory. Let’s consider thus the situation described by:

s

→ sink 2-53

The rate equation which describes the number of remaining defects in the metal is:

*

*- " s 2-54

The solution to this equation is:

" _{}^{"/0} 2-55

being the rate constant proportional to diffusion coefficient D and to a parameter α which contains the information related to the geometry of external surfaces or the concentration of dislocation (i.e. the fixed sink concentration):

s " α " s^{1"}^{ಾ}^{/ #3} 2-56
where K0 is a constant including the geometrical factor, the lattice parameter and the sink
distribution. Thus the solution of the random migration of single defects is:

" ^{"/}^{బ}456 1"ಾ/ #30 2-57

Anihilation and clustering

When interstitial and vacancy type of defects are present simultaneously in the crystal, their diffusion can lead them to annihilate each other:

V s

→ >vw>-@ 2-58

The rate equation for n-type of defects is:

*D

*- " sD^{}D, 2-59

In an irradiation experiments when initial concentrations of vacancies and interstitials are equal, the number of interstitials that have disappear must equal the number of the vacancies destroyed, ci = ci0 - cV0+ cV and the rate of decay of the defects can be described by a simple second order equation:

*D

*- " sD^{}^{} 2-60

Note that in a more generic situation the decay of vacancy concentration is not necessarily equal to the interstitials decay and thus the order of the reaction wouldn’t be 2.

In the case of clustering a similar process would occur but including not only the possibility of binding but also a backward process of dissociation. A generic example of the process and the partial differential equation is indicated in eqns. 2-49 and 2-50.

Generic Rate equation

The order of the reaction is important to interpret the annealing process, since every single activated process is described by the generic chemical rate equation:

*

*- " s^{},
^{1"}^{ಾ}^{/ #3} 2-61

Where F(n) = n^{γ} is any continuous function of n and γ is the order of the equation.

Diffusion to sinks was a first order reaction, and i-V annihilation was a reaction of order two.

### Resistivity recovery method 2.4.

When a sample containing irradiation defects is gradually warmed at a constant rate of heating (h), the defects undergo diffusion and at suitable temperature intervals recombination stages, in which also trapping, diffusion to sinks and clustering can happen.

The residual resistivity is a property related to the number of defects, as indicated in equation 2-45. When the increasing heating is made in steps, the residual resistivity can be monitored (at low temperatures), and thus the defect concentrations. This process is called isochronal annealing. In such experimental conditions the constant rate of heating allows to relate time and temperature by the relation: T=ht. In the simplest picture it can be considered that every stage corresponds to a single activation process with constant activation energy. The defect concentration will decay with increasing temperature as described in equation 2-57, a graphical representation is provided in Fig. 2-8. The diffusion rate which follows the Arrhenius law increases rapidly with temperature, as qualitatively depicted in Fig. 2-9. By a simple change in variable, the time evolution of defect population can be expressed as a temperature evolution. From equation 2-61 now it follows that:

*

* ∝
^{1"}^{ಾ}^{/ #3} 2-62

A graphical solution provides easier visualization of what happens with defects given that equation 2-62 will be the result of multiplying the defect population (as a function of

temperature) times the diffusion rate, giving for the reaction rate a peak at a characteristic annealing temperature, Ta. The annealing peak is depicted in Fig. 2-10.

In a real RR experiment, the residual resistivity is increased by particle irradiation.

The irradiation is followed by an isochronal annealing process while the residual resistivity is monitored at every step. For the sake of clarity a graphical description of the experimental method is provided in Fig. 2-11. Along this thermal process the created defects will gain enough thermal energy to diffuse and annihilate or clusterize or even dissociate at high temperatures. Thus, though the different processes and equations previously showed, the residual resistivity of the irradiated sample might eventually recover its original value (non-irradiated residual resistivity) as the temperature is increased and most of the defects are recombined. This provides the overall RR curve containing all this information. If the steps of the annealing are close enough the derivative of the resistivity with temperature can be depicted and the appearance of peaks might reveal recovery stages in the so-called RR rate curve (or RR derivative). A schematic representation of RR kinetic processes in pure Fe and its recovery peaks as a function of defect population evolution taken from Fu et al. is indicated in Fig. 2-12 and Fig. 2-13. The recovery stages associated to different species diffusion and recombination are called stages ID2, IE, II and III.

Fig. 2-8: Defect population evolution, of a single diffusion process in isochronal annealing experiment.

Fig. 2-9: Rate diffusion evolution as isochronal annealing goes.

0 0,2 0,4 0,6 0,8 1 1,2

20 40 60 80 100 120 140 160 180

Defect concentration

Annealing temperature (K)

0 0,005 0,01 0,015 0,02

20 40 60 80 100 120 140 160 180

Rate Diffusion Constant (a.u.)

Annealing temperature (K)

Fig. 2-10: Annealing peak characteristic of a recombination process.

Fig. 2-11: RR experimental method: illustration of temperature ramps and resistivity measurements along isochronal annealing. Heating rate (10 K/min).

0
1 10^{-4}
2 10^{-4}
3 10^{-4}
4 10^{-4}
5 10^{-4}
6 10^{-4}

20 40 60 80 100 120 140 160 180

-dn/dT

Annealing temperature (K) Ta

Fig. 2-12: RR stages after electron irradiation. Schematic representation of the different recovery stages as a function of increasing annealing temperature and associated mechanisms as proposed in electron irradiated iron by Takaki et al. [24,39]. The labels I, I2

and squares represent mono- and di-interstitials and vacancies respectively.

Fig. 2-13: Simulated RR peaks and defect population evolution along isochronal annealing after electron irradiation. Upper graph shows the derivative with respect to temperature of the simulated RR showing the recovery stages identified by peaks. Green arrows indicate the

positions of the experimental peaks. Below 140 K, the curve was scaled down by a factor of
50 to reduce the intensity of stages. The lower graph depicts the associated defect
population evolution (for 16 x 10^{9} atoms). The magenta dashed arrows indicate the stage
positions in the simulation. The concentrations of clusters V3 and V4 are negligible: these
defects disappear almost immediately after they are formed because of their low migration

energies.

### Improved RR Method 2.5.

The above explained RR experimental method, which is basically based on low-temperature irradiation followed by subsequent annealing, works very well when studying defect kinetics of pure metals or the effect of impurities on such kinetics.

Nevertheless in the case of concentrated alloys the long range migration of defects is going to enhance re-arrangement of solutes within the alloy, as it has been introduced in section 2.1.4. As it is shown in equation 2-23 there is a linear relation between ρ and the SRO parameters. Thus the residual resistivity of a given concentrated alloy can be expressed as a function of different contributions:

' " '8 ' ' 2-63

being ρ0 the residual resistivity of the metal free of irradiation defects, ρD the resistivity contribution of point defects and ρS a contribution imposed by the SRO state. The term ρD

is proportional to the defect concentrations and its specific resistivity (as indicated in equation 2-45) whereas ρS was defined by Schülze and Lücke as [54]:

'" A 2-64

where B is a suitable constant with resistivity dimensions and s is a suitable dimensionless parameter which characterizes the degree of SRO.

Based on such description, the time evolution of the defects will induce two types of changes in the resistivity, one due to the migration of defects and other due to Cr rearrangement. The mechanism that might promote the short-range rearrangement of Cr atoms in the vicinity of trapped defects has been recently described and depicted by Nikolaev (Figs. 6 and 7 of [64]) for vacancy-carbon defects. The results obtained in the present thesis suggest that a similar mechanism with trapped I´s and V’s should operate in the case of non C-doped Fe-Cr samples. The mechanism suggested is depicted in Fig. 2-14 in the case of clustering. It can be seen that the long-range migration of vacancies is very effective changing SRO by Cr-Fe permutation reactions.

The effect of resistivity change enhance by SRO effects during isochronal annealing has been qualitatively depicted for systems supersaturated with only vacancies [48,50].

The case where the change of SRO produces an increase in resistivity is shown in Fig. 2-15.

Therefore, in a classical RR experiment preformed in a concentrated alloy it is expected to find the RR peaks distorted by variations of SRO, which might even change the sign of the slope of the RR curves (causing an increase of resistivity instead of a decrease, as it will be show in our results). Obviously this can mask or change the different recovery peaks due to pure defect recombinations (and therefore the interpretation of RR curve).

Indeed this side effect has almost not been considered and no solution has been provided up to now. In order to study such phenomena, and given that the kMC or Rate theory computational methods still cannot introduce the values of ρS contributions we have conceive a modification upon the traditional RR method which might be able to eliminate the effects of SRO contributions to the RR curves.